Presentation on theme: "Making Sustainability Economic"— Presentation transcript:
1Making Sustainability Economic The Only Option that Will Deliver?Hobart, Tasmania, Australia where I liveI will have to race over some slides but the presentation is always downloadable from the net if you missed something.All I ask is that you think about what I am saying.John Harrison B.Sc. B.Ec. FCPA.
2Sustainability Requires a Holistic Approach Our approach to sustainability and the most pressing problem of reducing CO2 in the air should be holistic and involve:Reductions in energy usage.Kyoto, energy rationing etc.Reductions in linkages to the environmentClosing loops, recycling etc.Massive sequestrationGeological sequestration, mineral sequestration and stopping de-afforestation.Of the above massive sequestration is politically easiest to implement and could potentially be an economic process.There is huge scope for sequestration and conversion of waste to resource in the built environment given the massive size of the materials flows involved.
3Economically Driven Sustainability In the past it was considered that economic development was linked to.growth in use of resources and energy.Population growth.We now understand that change itself is a stimulant for economic growth.Consider the implications of changing to carbon compounds or materials containing carbon as building materials.The challenge is to harness human behaviours which underlay economic supply and demand phenomena by changing the technical paradigm in favour of making carbon dioxide a resource.
4Achieving Sustainable Sustainability Our goal should be:To make sustainability an economic process.To do this we need to induce changes in demand and supply reducing energy and resource usage and detrimental linkages with the planet.Through education induce cultural change to increase the demand for sustainability.Innovate to change the technical paradigm to deliver sustainability.TecEco tec, eco and enviro cements are innovative sustainability enabling technologies.
5Achieving Sustainability as an Economic Process Increase in demand/price ratio for sustainability due to educationally induced cultural drift$SupplyGreater Sustainability and economic growthEquilibrium shiftDemandIncrease in supply/price ratio for more sustainable products due to innovative changes in the technical paradigm.#
6Techno Processes The technical paradigm Our linkages to the bio-geo-sphere are defined by techno processes describing and controlling the flow of matter and energy. It is these flows that have detrimental linkages to earth systems.technicalparadigmDetrimental affects on earth systems
7Earth SystemsAtmospheric composition, climate, land cover, marine ecosystems, pollution, coastal zones, freshwater systems, salinity and global biological diversity have all been substantially affected.
8There are Detrimental Affects Right Through the Techno Process Linkages that affect earth system flowsTake manipulate and make impactsEnd of lifecycle impactsUtility zoneGreater UtilityLess Utility
9To Make Carbon a Resource the Key is To Change the Technology Paradigm “By enabling us to make productive use of particular raw materials, technology determines what constitutes a physical resource1”Pilzer, Paul Zane, Unlimited Wealth, The Theory and Practice of Economic Alchemy, Crown Publishers Inc. New York.1990To change the technical paradigm we must change both supply and demand, both of which feedback on each other in such a way as to move the equilibrium towards sustainability.
10We Must Re-Invent Many Materials Take → Manipulate → Make → Use → Waste[ ←Materials→]What we take from the environment around us and how we manipulate and make materials out of what we take affects earth systems at both the take and waste ends of the techno-process.The techno-process controls:How much and what we have to take to manufacture the materials we use.How long materials remain of utility andWhat form they are in when we eventually throw them “away”.There is no such place as “away”, only a global commons
11Global Warming the Most Important Affect? Trend of global annual surface temperature relative to mean.
12Landfill – The Visible Legacy Landfill is the technical term for filling large holes in the ground with waste. Landfills release methane, can cause ill health in the area, lead to the contamination of land, underground water, streams and coastal waters and give rise to various nuisances including increased traffic, noise, odours, smoke, dust, litter and pests.
14Fixing the Techno - Function We need to change the techno function to:
15Fixing the Techno - Function And more desirably to:Recycling
16Recycling is Currently not Economic Recycling is substantially undertaken for costly “feel good” political reasons and unfortunately not driven by sound economicsMaking Recycling Economic Should be a Priority
17Recycling Materials = Reduced Emissions The above relationships hold true on a macro scale, provided we can change the technology paradigm to make the process of recycling much more efficient = economic.
19Recycling Can Involve Remixing e.g Blending of waste streams may be required to produce input materials below toxicity levels of various heavy metals
20Materials - the Key to Sustainability Materials are the key to our survival on the planet. The choice of materials controls emissions, lifetime and embodied energies, use of recycled wastes, maintenance of utility, recyclability and the properties of wastes returned to the bio-geo-sphere.
21Huge Potential for Sustainable Materials in the Built Environment The built environment is made of materials and is our footprint on earth.It comprises buildings and infrastructure.There are huge volumes involved. Building materials comprise70% of materials flows (buildings, infrastructure etc.)45% of waste that goes to landfill (15 % of new materials going to site are wasted.)improving the sustainability of materials used to create the built environment will reduce the impact of the take and waste phases of the techno-process.By including carbon, all materials are potentially carbon sinks.All materials we make should not leave the techno-sphereC
22The Largest Material Flow - Cement and Concrete Concrete made with cement is the most widely used material on Earth accounting for some 30% of all materials flows on the planet and % of all materials flows in the built environment.Global Portland cement production is in the order of 2 billion tonnes per annum.Globally over 14 billion tonnes of concrete are poured per year.That’s over 2 tonnes per person per annumTecEco Pty. Ltd. have benchmark technologies for improvement in sustainability and properties
23Embodied Energy of Building Materials Concrete is relatively environmentally friendly and has a relatively low embodied energyDownloaded from (last accessed 07 March 2000)
24Average Embodied Energy in Buildings Most of the embodied energy in the built environment is in concrete.But because so much is used there is a huge opportunity for sustainability by reducing the embodied energy, reducing the carbon debt (net emissions) and improving properties.Downloaded from (last accessed 07 March 2000)
25Emissions from Cement Production Portland cement used in construction is made from carbonate.The process of calcination involves driving off chemically bound CO2 with heat.CaCO3 →CaO + ↑CO2∆Heating also requires energy.Most energy is derived from fossil fuels.Fuel oil, coal and natural gas are directly or indirectly burned to produce the energy required releasing CO2.The production of cement for concretes accounts for around 10%(1) of global anthropogenic CO2.(1) Pearce, F., "The Concrete Jungle Overheats", New Scientist, 19 July, No 2097, 1997 (page 14).
27Innovative New Materials Vital It is possible to achieve Kyoto targets as the UK are proving, but we need to go way beyond the treaty according to our chief scientists.Carbon rationing has been proposed as the only viable means to keep the carbon dioxide concentration in the atmosphere below 450 ppm.Atmospheric carbon reduction is essential, but difficult to politically achieve by rationing.Making the built environment not only a repository for recyclable resources (referred to as waste) but a huge carbon sink is an alternative and adjunct that is politically viable as it potentially results in economic benefits.Concrete, a cementitous composite, is the single biggest material flow on the planet with over 2.2 tonnes per person produced.Eco-cements offer tremendous potential for capture and sequestration using cementitious composites.MgCO3 → MgO + ↓CO2 - Efficient low temperature calcination & capture MgO + ↓CO2 + H2O → MgCO3.3H2O - Sequestration as building material ∆
30TecEco Binders– A Blending System TecEco concretes are a system of blending reactive magnesia, Portland cement and usually a pozzolan with other materials and are a key factor for sustainability.
31TecEco Formulations Tec-cements (5-10% MgO, 90-95% OPC) contain more Portland cement than reactive magnesia. Reactive magnesia hydrates in the same rate order as Portland cement forming Brucite which uses up water reducing the voids:paste ratio, increasing density and possibly raising the short term pH.Reactions with pozzolans are more affective. After all the Portlandite has been consumed Brucite controls the long term pH which is lower and due to it’s low solubility, mobility and reactivity results in greater durability.Other benefits include improvements in density, strength and rheology, reduced permeability and shrinkage and the use of a wider range of aggregates many of which are potentially wastes without reaction problems.Eco-cements (15-90% MgO, 85-10% OPC)contain more reactive magnesia than in tec-cements. Brucite in porous materials carbonates forming stronger fibrous mineral carbonates and therefore presenting huge opportunities for waste utilisation and sequestration.Enviro-cements (15-90% MgO, 85-10% OPC)contain similar ratios of MgO and OPC to eco-cements but in non porous concretes brucite does not carbonate readily.Higher proportions of magnesia are most suited to toxic and hazardous waste immobilisation and when durability is required. Strength is not developed quickly nor to the same extent.
32Why Reactive Magnesia?One of the most important variables in concretes affecting most properties is water.The addition of reactive magnesia has profound affects on both the fluid properties of water and the amount of water remaining in the mix during setting.Corrosion texts describe the protective role of brucite.The consequences of putting brucite through the matrix of a concrete in the first place need to be considered.Reactive MgO is a new tool to be understood with profound affects on most properties
33Sustainability The Current Technical Driection Reduce the amount of total binder.Use more supplementary materialsPfa, gbfs, industrial pozzolans etc.Use of recycled aggregates.Including aggregates containing carbonThe use of MgO potentially overcomes:Problems using acids to etch plastics so they bond with concretes.Problem of sulphates from plasterboard etc. ending up in recycled construction materials.Problems with heavy metals and other contaminants.Problems with delayed reactivity e.g. ASR with glass culletEco-cements further provide carbonation of the binder component.Possibility of easy capture of CO2 during the manufacturing process.Enhanced by using reactive MgO
34TecEco Kiln Technology Grinds and calcines at the same time.Runs 25% to 30% more efficiency.Can be powered by solar energy or waste heat.Brings mineral sequestration and geological sequestration togetherCaptures CO2 for bottling and sale to the oil industry (geological sequestration).The products – CaO &/or MgO can be used to sequester more CO2 and then be re-calcined. This cycle can then be repeated.Suitable for making reactive reactive MgO.
35Making Recycling Economic Reducing, re-using and recycling is done more for feel good reasons than good economics and costs the community heaps!To get over the laws of increasing returns and economies of scale and to make the sorting of wastes economic so that wastes become low cost inputs for the techno-process new technical paradigms are required. The way forward involves at least:A new killer technology in the form of a method for sorting wastes. (See TecEco web site for more details)A killer application for unsorted wastes.TecEco cements are a low pH benign environment suitable for hosting many wastes
36A Killer Application for Waste? WastesUtilizing wastes based on their chemical composition involves energy consuming transport.Wastes could be utilized as resources depending on their class of properties rather than chemical composition.in vast quantities based on broadly defined properties such as light weight, tensile strength, insulating capacity, strength or thermal capacity in composites.Many wastes contain carbon and if utilized would result in net carbon sinks.TecEco binders enable wastes to be converted to resources. Two examples:Plastics are currently hard to recycle because to be reused as manufacturing inputs they cannot usually be mixed. Yet they would impart light weight and insulating properties to a composite bound with the new carbon dioxide absorbing TecEco eco-cements.Sawdust and wood waste is burned in the bush contributing to global CO2. If taken to the tip, methane, which is worse is the end result. Yet wood waste it light in weight, has tensile strength, captured in a mineral binder is a carbon sink and provides excellent insulation.
37The Impact of TecEco Technology TecEco magnesian cement technology will be pivotal in bringing about sustainability in the built environment.Tec-Cements Develop Significant Early Strength even with Added Supplementary Materials. Around 25 = 30% less binder is required for the same strength.Eco-cements carbonate sequestering CO2Both tec and eco=cements provide a benign low pH environment for hosting large quantities of wasteThe CO2 released by calcined carbonates used to make binders can be captured using TecEco kiln technology.
38Our Dream - TecEco Cements for Sustainable Cities
39Robotics Will Result in Greater Sustainability Construction in the future will be largely achieved using robots. Like a color printer different materials will be required for different parts of structures, and wastes such as plastics will provide many of the properties required for the cementitious composites used. A non-reactive binder such as TecEco tec-cements will supply the right rheology and environment, and as with a printer, there will be very little waste.
40TecEco Binders - Solving Waste Problems An important objective should be to make cementitious composites that can utilise wastes.TecEco cements provide a benign environment suitable for waste immobilisation.Many wastes such as fly ash, sawdust , shredded plastics etc. can improve a property or properties of the cementitious composite.There are huge materials flows in both wastes and building and construction. TecEco technology leads the world in the race to incorporate wastes in cementitous composites
41TecEco Binders - Solving Waste Problems (2) If wastes are not immobile they should be immobilised.TecEco cementitious composites represent a cost affective option for both use and immobilisation.TecEco technology is more suitable than either lime, Portland cement or Portland cement lime mixes because of:Lower reactivity (less water, lower pH)Reduced solubility of heavy metals (lower pH)Greater durabilityDense, impermeable andHomogenous.No bleed waterAre not attacked by salts in ground or sea waterAre dimensionally more stable with less crackingTecEco cements are more predictable and easier to use than geopolymers.
42Why TecEco Binders are Excellent for Toxic and Hazardous Waste Immobilisation In a Portland cement brucite matrixOPC takes up lead, some zinc and germaniumBrucite and hydrotalcite are both excellent hosts for toxic and hazardous wastes.Heavy metals not taken up in the structure of Portland cement minerals or trapped within the brucite layers end up as hydroxides with minimal solubility.The brucite in TecEco cements has a structure comprising electronically neutral layers and is able to accommodate a wide variety of extraneous substances between the layers and cations of similar size substituting for magnesium within the layers and is known to be very suitable for toxic and hazardous waste immobilisation.
43Lower Solubility of Metal Hydroxides There is a 104 difference
45Embodied Energy and Emissions Energy costs money and results in emissions and is the largest cost factor in the production of mineral binders.Whether more or less energy is required for the manufacture of reactive magnesia compared to Portland cement or lime depends on the stage in the utility adding process it is measured.Utility is greatest in the finished product which is concrete. The volume of built material is more relevant than the mass and is therefore more validly compared. On this basis the technology is far more sustainable than either the production of lime or Portland cement.The new TecEco kiln technology will result in around 25% less energy being required and the capture of CO2 during production will result in less energy, lower costs and carbon credits.The manufacture of reactive magnesia is a benign process that can be achieved with waste or intermittently available energy.
46Energy – On a Mass Basis CaCO3 + Clay 1545.73 2828.69 Portland Cement Relative to Raw Material Used to make CementFrom Manufacturing Process Energy Release 100% Efficient (MJ.tonne-1)From Manufacturing Process Energy Release with Inefficiencies (MJ.tonne-1)Relative Product Used in CementRelative to Mineral Resulting in CementCaCO3 + ClayPortland Cement1807Hydrated OPCCaCO3Ca(OH)2MgCO3MgOMg(OH)2
47Energy – On a Volume Basis Relative to Raw Material Used to make CementFrom Manufacturing Process Energy Release 100% Efficient (MJ.metre-3)From Manufacturing Process Energy Release with Inefficiencies (MJ.metre-3)Relative Product Used in CementRelative to Mineral Resulting in CementCaCO3 + ClayPortland CementHydrated OPCCaCO3Ca(OH)2MgCO3MgOMg(OH)2
48Global AbatementWithout CO2 Capture during manufacture (billion tonnes)With CO2 Capture during manufacture (billion tonnes)Total Portland Cement Produced Globally1.80Global mass of Concrete (assuming a proportion of 15 mass% cement)12.00Global CO2 Emissions from Portland Cement3.60Mass of Eco-Cement assuming an 80% Substitution in global concrete use9.60Resulting Abatement of Portland Cement CO2 Emissions2.88CO2 Emissions released by Eco-Cement2.591.34Resulting Abatement of CO2 emissions by Substituting Eco-Cement0.291.53
49Abatement from Substitution Building Material to be substitutedRealistic % Subst-itution by TecEco technologySize of World Market (million tonnesSubstituted Mass (million tonnes)CO2 Factors (1)Emission From Material Before SubstitutionEmission/Sequestration from Substituted Eco-Cement (Tonne for Tonne Substitution Assumed)Net AbatementEmissions - No CaptureEmissions - CO2 CaptureAbatement - No CaptureAbatement CO2 CaptureBricks85%250212.50.2859.522.214.171.1249.8Steel25%8402102.38499.856.629.4443.2470.4Aluminium20%20.54.118.073.81.10.672.773.2TOTAL426.620.7633.1114.959.7518.2573.4Concretes already have low lifetime energies.If embodied energies are improved could substitution mean greater market share?Figures are in millions of Tonnes
50Sustainability Issues Summary We will not kick the fossil fuel habit. It will kick us when we run out of fuel. Sequestration on a massive scales is therefore essential.To reduce our linkages with the environment we must recycle.Sequestration and recycling have to be economic processes or they have no hope of success.We cannot stop progress, but we can change and historically economies thrive on change.What can be changed is the technical paradigm. CO2 and wastes need to be redefined as resources.New and better materials are required that utilize wastes including CO2 to create a wide range of materials suitable for use in our built environment.
51Policy Message Summary Governments cannot easily legislate for sustainability, it is more important that ways are found to make sustainability good business.“Feel good” legislation does not work.EPR Legislation works but is difficult to implement successfully.Carbon rationing would be difficult to achieve globally.It is therefore important for governments to make efforts to understand new technical paradigms that will change the techno-process so it delivers sustainable outcomesMaterials are the new frontier of technologyEmbedded intelligence enabling sorting should be globally standardized.Robotics are inevitable - we need to be prepared.Cementitious composites can redefine wastes as resources and sequester CO2.“The TecEco Technology Must be Developed” was a finding of the recent ISOS Conference.
52Limiting Factors for Development of TecEco Technology Credibility Issues that can only be overcome with significant funded research by TecEco and third parties.Economies of scaleGovernment procurement policiesSubsidies for materials that can demonstrate clear sustainable advantages.Carbon taxes/credits.Formula rather than performance based standardsFormula based standards enshrine mediocrity and the status quo.A legislative framework enforcing performance based standards is essential.For example cement standards excluding magnesium are based on historical misinformation and lack of understanding.
53There is no End with TecEco Technology – Only a Beginning. More technical slides follow
54TecEco Cements– A Blending System TecEco cementitious composites are a system of blending reactive magnesia, Portland cement and usually a pozzolan with other materials.
55TecEco Formulations Tec-cements (5-10% MgO, 90-95% OPC) contain more Portland cement than reactive magnesia. Reactive magnesia hydrates in the same rate order as Portland cement forming Brucite which uses up water reducing the voids:paste ratio, increasing density and possibly raising the short term pH.Reactions with pozzolans are more affective. After all the Portlandite has been consumed Brucite controls the long term pH which is lower and due to it’s low solubility, mobility and reactivity results in greater durability.Other benefits include improvements in density, strength and rheology, reduced permeability and shrinkage and the use of a wider range of aggregates many of which are potentially wastes without reaction problems.Eco-cements (15-90% MgO, 85-10% OPC)contain more reactive magnesia than in tec-cements. Brucite in porous materials carbonates forming stronger fibrous mineral carbonates and therefore presenting huge opportunities for waste utilisation and sequestration.Enviro-cements (15-90% MgO, 85-10% OPC)contain similar ratios of MgO and OPC to eco-cements but in non porous concretes brucite does not carbonate readily.Higher proportions of magnesia are most suited to toxic and hazardous waste immobilisation and when durability is required. Strength is not developed quickly nor to the same extent.
56Strength with Blend & Porosity Tec-cement concretesEco-cement concretesHigh PorosityEnviro-cement concretesHigh OPCHigh MagnesiaSTRENGTH ON ARBITARY SCALE 1-100
57Consequences of replacing Portlandite with Brucite Portlandite (Ca(OH)2) is too soluble, mobile and reactive. It carbonates readily and being soluble can act as an electrolyte.TecEco generally remove Portlandite using the pozzolanic reaction and add reactive magnesia which hydrates forming brucite which is another alkali, but much less soluble, mobile or reactive than Portlandite.The consequences of removing Portlandite (Ca(OH)2 with the pozzolanic reaction and filling the voids between hydrating cement grains with Brucite Mg(OH)2, an insoluble alkaline mineral, need to be considered.
58TecEco Technology - Simple Yet Ingenious? The TecEco technology demonstrates that magnesia, provided it is reactive rather than “dead burned” (or high density, periclase type), can be beneficially added to cements in excess of the amount of 5 mass% generally considered as the maximum allowable by standardsNote that dead burned magnesia is much less expansive than dead burned lime (Ramachandran V. S., Concrete Science, Heydon & Son Ltd. 1981, p )Reactive magnesia is essentially amorphous magnesia with low lattice energy.It is produced at low temperatures and finely ground, andwill completely hydrate in the same time order as the minerals contained in most hydraulic cements.Dead burned magnesia and lime have high lattice energiesDo not hydrate rapidly andcause dimensional distress.
59Summary of Reactions Involved We think the reactions are relatively independent.Notice the low solubility of brucite compared to Portlandite and that nesquehonite adopts a more ideal habit than calcite & aragonite
60Tec-Cements-Less Binder for the Same Strength. Concretes are more often than not made to strength.The use of tec-cement results in20-30% greater strength or less binder for the same strength.more rapid strength development even with added pozzolans.
61Reasons for Strength Development in Tec-Cements. Reactive magnesia requires considerable water to hydrate resulting in:Denser, less permeable concrete.A significantly lower voids/paste ratio.Higher early pH initiating more effective silicification reactions?The Ca(OH)2 normally lost in bleed water is used internally for reaction with pozzolans.Super saturation of alkalis caused by the removal of water?Micro-structural strength due to particle packing (Magnesia particles at 4-5 micron are about 1/8th the size of cement grains.)Slow release of water from around highly charged Mg++ ion?
62Water Reduction During the Plastic Phase Water is required to plasticise concrete for placement, however once placed, the less water over the amount required for hydration the better. Magnesia consumes water as it hydrates producing solid material.Less water results in less shrinkage and cracking and improved strength and durability. Concentration of alkalis and increased density result in greater strength.
63Tec-Cement Compressive Strength Graphs by Oxford Uni Student
64Tec-Cement Tensile Strength Graphs by Oxford Uni Student
65Other Strength Testing to Date BRE (United Kingdom)2.85PC/0.15MgO/3pfa(1 part) : 3 parts sand - Compressive strength of 69MPa at 90 days.Note that there was as much pfa as Portland cement plus magnesia. Strength development was consistently greater than the OPC controlTecEcoThe mix was:Portland cement245 Kg10.88%12.29%Magnesia30 Kg1.39%Fly ash70 Kg3.24%Quarry dust215 Kg9.55%White sand550 Kg25.46%Dolerate aggregate1060 Kg49.07%
66Tec-Cement Concrete Strength Gain Curve The possibility of strength gain with less cement and added pozzolans is of great economic and environmental importance.
67A Few Warnings About Trying to Repeat TecEco Findings with Tec-Cements MgO is a fine powder and like other fine powders has a high water demand so the tendency is to add too much water. As for other concretes this significantly negatively impacts on strength.Mg++ when it goes into solution is a small atom with a high charge and tends to affect water molecules which are polar. The result is a Bingham plastic quality which means energy is required to introduce a shear thinning to allow placement.Do not use the slump test!With ordinary Portland cement concretes as rheology prior to placement is observed in the barrel of a concrete truck whilst energy is applied by the revolving barrel.Is what is done in practice more accurate that the slump test anyway?
68Eco-Cement Strength Development Eco-cements gain early strength from the hydration of OPC. Later strength comes from the carbonation of brucite forming an amorphous phase, lansfordite and nesquehonite.Strength gain is mainly microstructural because ofMore ideal particle packing (Brucite particles at 4-5 micron are about 1/8th the size of cement grains.)The natural fibrous and acicular shape of magnesium carbonate minerals which tend to lock together.
69Eco-Cement Concrete Strength Gain Curve Eco-cement bricks, blocks, pavers and mortars etc. take a while to come to the same or greater strength than OPC formulations but are stronger than lime based formulations.
71Proof of Carbonation - Minerals Present After 18 Months XRD showing carbonates and other minerals before removal of carbonates with HCl in a simple Mix (70 Kg PC, 70 Kg MgO, colouring oxide .5Kg, sand unwashed 1105 Kg)
72Proof of Carbonation - Minerals Present After 18 Months and Acid Leaching XRD Showing minerals remaining after their removal with HCl in a simple mix (70 Kg PC, 70 Kg MgO, colouring oxide .5Kg, sand unwashed 1105 Kg)
73A Few Warnings About Trying to Repeat TecEco Findings with Eco-Cements Eco-cements will only gain strength in materials that are sufficiently porous to allow the free entry of CO2.Testing in accordance with standards designed for hydraulic cements is irrelevant.There appears to be a paucity of standards that apply to carbonating lime mortars however we understand the European Lime project will rectify this.Most knowledge of carbonating materials is to be found amongst the restoration fraternity.Centuries of past experience and good science dictate well graded aggregates with a coarser fraction for sufficient porosity. These are generally found in concrete blocks made to today’s standards but not in mortars.
74Increased Density – Reduced Permeability Concretes have a high percentage (around 18%) of voids.On hydration magnesia expands % filling voids and surrounding hydrating cement grains.Brucite is mass% water.On carbonation to nesquehonite brucite expands 307%Nesquehonite is % water and CO2Cheap binder!!!Lower voids:paste ratios than water:binder ratios result in little or no bleed water less permeability and greater density.Compare the affect to that of vacuum dewatering.
75Reduced PermeabilityAs bleed water exits ordinary Portland cement concretes it creates an interconnected pore structure that remains in concrete allowing the entry of aggressive agents such as SO4--, Cl- and CO2TecEco tec - cement concretes are a closed system. They do not bleed as excess water is consumed by the hydration of magnesia.As a result TecEco tec - cement concretes dry from within, are denser and less permeable and therefore stronger more durable and more waterproof. Cement powder is not lost near the surfaces. Tec-cements have a higher salt resistance and less corrosion of steel etc.
78A Lower More Stable Long Term pH In TecEco cements the long term pH is governed by the low solubility and carbonation rate of brucite and is much lower at around , allowing a wider range of aggregates to be used, reducing problems such as AAR and etching. The pH is still high enough to keep Fe3O4 stable in reducing conditions.Eh-pH or Pourbaix Diagram The stability fields of hematite, magnetite and sideritein aqueous solution; total dissolved carbonate = 10-2M.Steel corrodes below 8.9
79Reduced Delayed Reactions A wide range of delayed reactions can occur in Portland cement based concretesDelayed alkali silica and alkali carbonate reactionsThe delayed formation of ettringite and thaumasiteDelayed hydration of minerals such as dead burned lime and magnesia.Delayed reactions cause dimensional distress and possible failure.
80Reduced Delayed Reactions (2) Delayed reactions do not appear to occur to the same extent in TecEco cements.A lower long term pH results in reduced reactivity after the plastic stage.Potentially reactive ions are trapped in the structure of brucite.Ordinary Portland cement concretes can take years to dry out however the reactive magnesia in Tec-cement concretes consumes unbound water from the pores inside concrete.Reactions do not occur without water.
81CarbonationCarbonates are the stable phases of both calcium and magnesium.Carbonation in the built environment would result in significant sequestration because of the shear volumes involved.The formation of carbonates lowers the pH of concretes compromising the stability of the passive oxide coating on steel.Carbonation adds considerable strength and some steel reinforced structural concrete could be replaced with fibre reinforced porous carbonated concrete.
82Carbonation (2) Gor nesquehonite to magnesite = 8.56 kJ.mol-1 There are a number of carbonates of magnesium. The main ones appear to be an amorphous phase, lansfordite and nesquehonite.Gor Brucite to nesquehonite = kJ.mol-1Compare to Gor Portlandite to calcite = kJ.mol-1The dehydration of nesquehonite to form magnesite is not favoured by simple thermodynamics but may occur in the long term under the right conditions.Gor nesquehonite to magnesite = 8.56 kJ.mol-1But kinetically driven by desiccation during drying.Reactive magnesia can carbonate in dry conditions – so keep bags sealed!For a full discussion of the thermodynamics see our technical documents.TecEco technical documents on the web cover the important aspects of carbonation.
83Ramifications of Carbonation Magesium Carbonates.The magnesium carbonates that form at the surface of tec – cement concretes expand significantly thereby sealing off further carbonation.Lansfordite and nesquehonite are formed in porous eco-cement concrete as there are no kinetic barriers. Lansfordite and nesquehonite are stronger and more acid resistant than calcite or aragonite.The curing of eco-cements in a moist - dry alternating environment seems to encourage carbonation via Lansfordite and nesquehonite .Carbonation results in a fall in pH.Portland Cement ConcretesCarbonation proceeds relatively rapidly at the surface. ?Vaterite? followed by Calcite is the principal product and lowers the pH to around 8.2
84Reduced ShrinkageNet shrinkage is reduced due to stoichiometric expansion of Magnesium minerals, and reduced water loss.Dimensional change such as shrinkage results in cracking and reduced durability
85Reduced Shrinkage – Less Cracking Cracking, the symptomatic result of shrinkage, is undesirable for many reasons, but mainly because it allows entry of gases and ions reducing durability. Cracking can be avoided only if the stress induced by the free shrinkage strain, reduced by creep, is at all times less than the tensile strength of the concrete. Tec-cements may also have greater tensile strength.Reduced in TecEco tec-cements.After Richardson, Mark G. Fundamentals of Durable Reinforced Concrete Spon Press, page 212.
86Durability - Reduced Salt & Acid Attack Brucite has always played a protective role during salt attack. Putting it in the matrix of concretes in the first place makes sense.Brucite does not react with salts because it is a least 5 orders of magnitude less soluble, mobile or reactive.Ksp brucite = 1.8 X 10-11Ksp Portlandite = 5.5 X 10-6TecEco cements are more acid resistant than Portland cementThis is because of the relatively high acid resistance (?) of Lansfordite and nesquehonite compared to calcite or aragonite
87Improved WorkabilityFinely ground reactive magnesia acts as a plasticiserThere are also surface charge affects
88Bingham Plastic Rheology It is not known how deep these layers getThe strongly positively charged small Mg++ atoms attract water which is polar in deep layers affecting the rheological properties.Etc.Etc.Ca++ = 114, Mg++ = 86 picometres
89Rheology TecEco concretes and mortars are: Very homogenous and do not segregate easily. They exhibit good adhesion and have a shear thinning property.Exhibit Bingham plastic qualities and react well to energy input.Have good workability.TecEco concretes with the same water/binder ratio have a lower slump but greater plasticity and workability.TecEco tec-cements are potentially suitable for mortars, renders, patch cements, colour coatings, pumpable and self compacting concretes.A range of pumpable composites with Bingham plastic properties will be required in the future as buildings will be “printed.”
90Robotics Will Result in Greater Sustainability Construction in the future will be largely achieved using robots. Like a color printer different materials will be required for different parts of structures, and wastes such as plastics will provide many of the properties required for the cementitious composites used. A non-reactive binder such as TecEco tec-cements will supply the right rheology and environment, and as with a printer, there will be very little waste.
91Dimensionally Control Over Concretes During Curing? Portland cement concretes shrink around .05%. Over the long term much more (>.1%).Mainly due to plastic and drying shrinkage.The use of some wastes as aggregates causes shrinkage e.g. wood waste in masonry units, thin panels etc.By varying the amount and form of magnesia added dimensional control can be achieved.
92Volume Changes on Hydration When magnesia hydrates it expands:MgO (s) + H2O (l) ↔ Mg(OH)2 (s)↔ molar massliquid ↔ molar volumesUp to % solidus expansion depending on whether the water is coming from stoichiometric mix water, bleed water or from outside the system. In practice much less as the water comes from mix and bleed water.The molar volume (L.mol-1)is equal to the molar mass (g.mol-1) divided by the density (g.L-1).
93Volume Changes on Carbonation Consider what happens when Portlandite carbonates:Ca(OH)2 + CO2 CaCO3↔ 100 molar massgas ↔ molar volumesSlight expansion. But shrinkage from surface water lossCompared to brucite forming nesquehonite as it carbonates:Mg(OH)2 + CO2 MgCO3.3H2O↔ molar massgas ↔ molar volumes307 % expansion (less water volume reduction) and densification of the surface preventing further ingress of CO2 and carbonation. Self sealing?The molar volume (L.mol-1)is equal to the molar mass (g.mol-1) divided by the density (g.L-1).
94TecEco Cement Concretes –Dimensional Control Combined – Hydration and Carbonation can be manipulated to be close to neutral.So far we have not observed shrinkage in TecEco tec - cement concretes (5% -10% substitution OPC) also containing fly ash.At some ratio, thought to be around 5% -10% reactive magnesia and 90 – 95% OPC volume changes cancel each other out.The water lost by Portland cement as it shrinks is used by the reactive magnesia as it hydrates eliminating shrinkage.Note that brucite is mass% water, nesquehonite is 243 mass% water and CO2It makes sense to make binders out of CO2 and water!.More research is required for both tec - cements and eco-cements to accurately establish volume relationships.The molar volume (L.mol-1)is equal to the molar mass (g.mol-1) divided by the density (g.L-1).
96Reduced Steel Corrosion Steel remains protected with a passive oxide coating of Fe3O4 above pH 8.9.A pH of over 8.9 is maintained by the equilibrium Mg(OH)2 ↔ Mg++ + 2OH- for much longer than the pH maintained by Ca(OH)2 because:Brucite does not react as readily as Portlandite resulting in reduced carbonation rates and reactions with salts.Concrete with brucite in it is denser and carbonation is expansive, sealing the surface preventing further access by moisture, CO2 and salts.Brucite is less soluble and traps salts as it forms resulting in less ionic transport to complete a circuit for electrolysis and less corrosion.Free chlorides and sulfates originally in cement and aggregates are bound by magnesiumMagnesium oxychlorides or oxysulfates are formed. ( Compatible phases in hydraulic binders that are stable provided the concrete is dense and water kept out.)
97Corrosion in Portland Cement Concretes Both carbonation, which renders the passive iron oxide coating unstable or chloride attack (various theories) result in the formation of reaction products with a higher electrode potential resulting in anodes with the remaining passivated steel acting as a cathode.Passive Coating Fe3O4 intactCorrosionAnode: Fe → Fe+++ 2e- Cathode: ½ O2 + H2O +2e- → 2(OH)- Fe++ + 2(OH)- → Fe(OH)2 + O2 → Fe2O3 and Fe2O3.H2O (iron oxide and hydrated iron oxide or rust)The role of chloride in CorrosionAnode: Fe → Fe+++ 2e- Cathode: ½ O2 + H2O +2e- → 2(OH)- Fe++ +2Cl- → FeCl2 FeCl2 + H2O + OH- → Fe(OH)2 + H+ + 2Cl- Fe(OH)2 + O2 → Fe2O3 and Fe2O3.H2OIron hydroxides react with oxygen to form rust. Note that the chloride is “recycled” in the reaction and not used up.
98Less Freeze - Thaw Problems Denser concretes do not let water in.Brucite will to a certain extent take up internal stressesWhen magnesia hydrates it expands into the pores left around hydrating cement grains:MgO (s) + H2O (l) ↔ Mg(OH)2 (s)↔ molar mass↔ molar volumes↔ molar volumes38% air voids are created in space that was occupied by magnesia and water!Air entrainment can also be used as in conventional concretesTecEco concretes are not attacked by the salts used on roads
99TecEco Binders - Solving Waste Problems There are huge volumes of concrete produced annually ( 2 tonnes per person per year )The goal should be to make cementitious composites that can utilise wastes.TecEco cements provide a benign environment suitable for waste immobilisationMany wastes such as fly ash, sawdust , shredded plastics etc. can improve a property or properties of the cementitious composite.There are huge materials flows in both wastes and building and construction. TecEco technology will lead the world in the race to incorporate wastes in cementitous composites
100TecEco Binders - Solving Waste Problems (2) If wastes are not immobile they should be immobilised.TecEco cementitious composites represent a cost affective option for both use and immobilisation.TecEco technology is more suitable than either lime, Portland cement or Portland cement lime mixes because of:Lower reactivity (less water, lower pH)Reduced solubility of heavy metals (lower pH)Greater durabilityDense, impermeable andHomogenous.No bleed waterAre not attacked by salts in ground or sea waterAre dimensionally more stable with less crackingTecEco cements are more predictable and easier to use than geopolymers.
101Role of Brucite in Immobilisation In a Portland cement brucite matrixOPC takes up lead, some zinc and germaniumBrucite and hydrotalcite are both excellent hosts for toxic and hazardous wastes.Heavy metals not taken up in the structure of Portland cement minerals or trapped within the brucite layers end up as hydroxides with minimal solubility.The brucite in TecEco cements has a structure comprising electronically neutral layers and is able to accommodate a wide variety of extraneous substances between the layers and cations of similar size substituting for magnesium within the layers and is known to be very suitable for toxic and hazardous waste immobilisation.
102Lower Solubility of Metal Hydroxides There is a 104 difference
103TecEco Materials are Fire Retardants The main phase in TecEco tec - cement concretes is Brucite.The main phases in TecEco eco-cements are Lansfordite and nesquehonite.Brucite, Lansfordite and nesquehonite are excellent fire retardants and extinguishers.At relatively low temperaturesBrucite releases water and reverts to magnesium oxide.Lansfordite and nesquehonite releases CO2 and water and convert to magnesium oxide.Fires are therefore not nearly as aggressive resulting in less damage to structures.Damage to structures results in more human losses that direct fire hazards.
104High Performance-Lower Construction Costs Less binders (OPC + magnesia) for the same strength.Faster strength gain even with added pozzolans.Elimination of shrinkage reducing associated costs.Elimination of bleed water enables finishing of lower floors whilst upper floors still being poured and increases pumpability.Cheaper binders as less energy requiredIncreased durability will result in lower costs/energies/emissions due to less frequent replacement.Because reactive magnesia is also an excellent plasticiser, other costly additives are not required for this purpose.A wider range of aggregates can be utilised without problems reducing transport and other costs/energies/emissions.
105TecEco Concretes - Lower Construction Costs (2) Homogenous, do not segregate with pumping or work.Easier placement and better finishing.Reduced or eliminated carbon taxes.Eco-cements can to a certain extent be recycled.TecEco cements utilise wastes many of which improve properties.Improvements in insulating capacity and other properties will result in greater utility.Products utilising TecEco cements such as masonry and precast products can in most cases utilise conventional equipment and have superior properties.A high proportion of brucite compared to Portlandite is water and of Lansfordite and nesquehonite compared to calcite is CO2.Every mass unit of TecEco cements therefore produces a greater volume of built environment than Portland and other calcium based cements. Less need therefore be used reducing costs/energy/emissions.
106TecEco Challenging the World The TecEco technology is new and not yet fully characterised.It offers sustainability in the built environment not previously considered possible.The world desperately needs a way of sequestering large volumes of CO2 such as made possible by eco-cements.Formula rather than performance based standards are preventing the development of new and better materials based on mineral binders.TecEco challenge universities governments and construction authorities to quantify performance in comparison to ordinary Portland cement and other competing materials.We at TecEco will do our best to assist.Negotiations are underway in many countries to organise supplies to allow such scientific endeavour to proceed.
107TecEco’s Immediate Focus TecEco will concentrate on:Killer applications that use a lot of cement, are easy to manage and that will initiate and achieve volume production.low technical risk products that require minimal research and development and for which performance based standards apply.Niche products for which our unique technology excels.Carbonated products such as bricks, blocks, stabilised earth blocks, pavers, roof tiles pavement and mortars that utilise large quantities of waste.Products where sustainability, rheology or fire retardation are required. (Mainly eco-cement technology using fly ash).Products such as oil well cement, gunnites, shotcrete, tile cements, colour renders and mortars where excellent rheology and bond strength are required.The immobilisation of wastes including toxic hazardous and other wastes because of the superior performance of the technology and the rapid growth of markets. (enviro and tec - cements).Controlled low strength materials e.g. mud bricks.Solving problems not adequately resolved using Portland cementProducts where extreme durability is required (e.g.bridge decking.)Products for which weight is an issue.
108TecEco Minding the Future TecEco are aware of the enormous weight of opinion necessary before standards can be changed globally for TecEco tec - cement concretes for general use.TecEco already have a number of institutions and universities around the world doing research.TecEco have publicly released the eco-cement technology and received huge global publicity.TecEco research documents are available from the TecEco web site by download, however a password is required. Soon they will be able to be purchased from the web site. .Other documents by other researchers will be made available in a similar manner as they become available.Technology standing on its own is not inherently good. It still matters whether it is operating from the right value system and whether it is properly available to all people.-- William Jefferson Clinton
109A Few Other Comments Research Business TecEco have found that in house research is difficult due to the high cost of equipment and lack of credibility of the results obtained.Although a large number of third party research projects have been initiated, the work has been slow due to inefficiencies and a lack of understanding of the technology. We are doing our best to address this with a new web site and a large number of papers and case histories that are being posted to it.TecEco are always keen to discuss research projects provided they are fair and the proposed test regime is appropriate.BusinessThere are significant business opportunities that are emerging particularly under the Clean Development Mechanism (CDM) of the Kyoto Protocol.TecEco are shifting the focus to tec-cement concretes due to economy of scale issues likely only to be overcome with the adoption of TecEco kiln technology and introduction of the superior Nichromet process (www.nichromet.com) to the processing of minerals containing Mg.Watch the development of robotic construction and placement without formwork as these new developments will require the use of binders with Bingham plastic qualities such as provided by TecEco technology.TecEco technology gives Mineral sequestration real economic relevance.
110Summary Simple, smart and sustainable? TecEco cement technology has resulted in potential solutions to a number of problems with Portland and other cements including durability and corrosion, the alkali aggregate reaction problem and the immobilisation of many problem wastes and will provides a range of more sustainable building materials.The right technology at the right time?TecEco cement technology addresses important triple bottom line issues solving major global problems with positive economic and social outcomes.Climate ChangePollutionDurabilityCorrosionStrengthDelayed ReactionsPlacement , FinishingRheologyShrinkageCarbon Taxes
111Characteristics of TecEco Cements (1) Portland Cement ConcretesTec-Cement ConcretesEnviro-Cement ConcretesEco-CementsTypical Formulations100 mass% PC8 mass% OPC, 72 mass % PC, 20 mass% pozzolan20 mass% OPC, 60 mass % PC, 20 mass% pozzolan50 mass% OPC, 30 mass % PC, 20 mass% pozzolanSettingMain strength from hydration of calcium silicates.Main strength is from hydration of calcium silicates. Magnesia hydrates forming brucite which has a protective role.Magnesia hydrates forming brucite which protects and hosts wastes. Carbonation is not encouraged.Magnesia hydrates forming brucite then carbonates forming Lansfordite and nesquehonite.SuitabilityDiverseDiverse. Ready mix concrete with high durabilityToxic and hazardous waste immobilisationBrick, block, pavers, mortars and renders.Mineral Assemblage (in cement)Tricalcium silicate, di calcium silicate, tricalcium aluminate and tetracalcium alumino ferrite.Tricalcium silicate, di calcium silicate, tricalcium aluminate, tetracalcium alumino ferrite, reactive magnesia.
112Characteristics of TecEco Cements (2) Portland Cement ConcretesTec-Cement ConcretesEnviro-Cement ConcretesEco-CementsFinal mineral Assemblage (in concrete)Complex but including tricalcium silicate hydrate, di calcium silicate hydrate, ettringite, monosulfoaluminate, (tetracalcium alumino sulphate), tricalcium alumino ferrite hydrate, calcium hydroxide and calcium carbonate .Complex but including tricalcium silicate hydrate, di calcium silicate hydrate, ettringite, monosulfoaluminate, (tetracalcium alumino sulphate), tricalcium alumino ferrite hydrate, calcium hydroxide, calcium carbonate, magnesium hydroxide and magnesium carbonates.StrengthVariable. Mainly dependent on the water binder ratio and cement content.Variable. Mainly dependent on the water binder ratio and cement content. Usually less total binder for the same strength developmentVariable, usually lower strength because of high proportion of magnesia in mix.Variable.
113Characteristics of TecEco Cements (3) Portland Cement ConcretesTec-Cement ConcretesEnviro-Cement ConcretesEco-CementsRate of Strength DevelopmentVariable. Addition of fly ash can reduce rate of strength development.Variable. Addition of fly ash does not reduce rate of strength development.Slow, due to huge proportion of magnesiaVariable, but usually slower as strength develops during carbonation process.pHControlled by Na+ and K+ alkalis and Ca(OH)2 in the short term. In the longer term pH drops near the surface due to carbonation (formation of CaCO3)Controlled by Na+ and K+ alkalis and Ca(OH)2 and high in the short term. Lower in the longer term and controlled by Mg(OH)2 and near the surface MgCO3High in the short term and controlled by Ca(OH)2. Lower in the longer term and controlled by MgCO3RheologyPlasticisers are required to make mixes workable.Plasticisers are not necessary. Formulations are generally much more thixotropic.Plasticisers are not necessary. Formulations are generally much more thixotropic and easier to use for block making.
114Characteristics of TecEco Cements (4) Portland Cement ConcretesTec-Cement ConcretesEnviro-Cement ConcretesEco-CementsDurabilityLack of durability is an issue with Portland cement concretesProtected by brucite, are not attacked by salts, do not carbonate, are denser and less permeable and will last indefinitely.Protected by brucite, are not attacked by salts, do not carbonate, are denser and will last indefinitely.DensityDensity is reduced by bleeding and evaporation of water.Do not bleed - water is used up internally resulting in greater densityPermeabilityPermeable pore structures are introduced by bleeding and evaporation of water.Do not bleed - water is used up internally resulting in greater density and no interconnecting pore structuresShrinkageShrink around %With appropriate blending can be made dimensionally neutral as internal consumption of water reduces shrinkage through loss of water and magnesium minerals are expansive.
115Characteristics of TecEco Cements (5) Portland Cement ConcretesTec-Cement ConcretesEnviro-Cement ConcretesEco-CementsInsulating PropertiesRelatively low with high thermal conductivity around 1.44 W/mKDepends on formulation but better insulation as brucite is a better insulatorDepends on formulation but better insulation as brucite is a better insulator and usually contains other insulating materialsThermal MassHigh. Specific heat is .84 kJ/kgKDepends on formulation but remains highEmbodied Energy (of concrete)Low, 20 mpa 2.7 Gj.t-1, 30 mpa 3.9 Gj.t-1 (1)Approx 15-30% lower due to less cement for same strength, lower process energy for making magnesia and high pozzolan content(2).Lower depending on formulation(2).Depends on formulation Even lower due to lower process energy for making magnesia and high pozzolan content(2).
116Characteristics of TecEco Cements (6) Portland Cement ConcretesTec-Cement ConcretesEnviro-Cement ConcretesEco-CementsRe-cyclabilityConcrete can only be crushed and recycled as aggregate.Can be crushed and recycled as aggregate.Can be crushed and fines re-calcined to produce more magnesia or crushed and recycled as aggregate or both.Fire RetardantCa(OH)2 and CaCO3 break down at relatively high temperatures and cannot act as fire retardantsMg(OH)2 is a fire retardant and releases H2O at relatively low temperatures.Mg(OH)2 and MgCO3 are both fire retardants and release H2O or CO2 at relatively low temperatures.
117Characteristics of TecEco Cements (7) Portland Cement ConcretesTec-Cement ConcretesEnviro-Cement ConcretesEco-CementsSustainabilityA relatively low embodied energy and emissions relative to other building products. High volume results in significant emissions.Less binder for the same strength and a high proportion of supplementary cementitous materials such as fly ash and gbfs. Can be formulated with more sustainable hydraulic cements such as high belite sulphoaluminate cements. A wider range of aggregates can be used. Greater durability.A high proportion of supplementary cementitous materials such as fly ash and gbfs. Can be formulated with more sustainable hydraulic cements such as high belite sulphoaluminate cements. A wider range of aggregates can be used. Greater durability.A high proportion of supplementary cementitous materials such as fly ash and gbfs. Carbonate in porous materials reabsorbing chemically released CO2A wider range of aggregates can be used. Greater durability.Carbon emissionsWith 15 mass% PC in concrete .32 t.t-1 After carbonation approximately .299 t.t-1With 15 mass% PC in concrete approx.29 t.t-1 After carbonation approximately .26 t.t-1 Could be lower using supplementary cementitous materials and formulated with other low carbon cement blends.With mass % magnesia and 3.75 mass % PC in concrete .241 t.t-1With capture CO2 and fly ash as low as .113 t.t-1